1 Journal of Colloid and Interface Science 280 (2004) The removal of heavy metal cations by natural zeolites E. Erdem a, N. Karapinar b,r.donat a, a Department of Chemistry, Faculty of Science and Arts, Pamukkale University, Denizli, Turkey b Department of Chemistry Engineering, Faculty of Engineering, Pamukkale University, Denizli, Turkey Received 24 March 2004; accepted 6 August 2004 Available online 25 September 2004 Abstract In this study, the adsorption behavior of natural (clinoptilolite) zeolites with respect to Co 2+,Cu 2+,Zn 2+,andMn 2+ has been studied in order to consider its application to purity metal finishing wastewaters. The batch method has been employed, using metal concentrations in solution ranging from 100 to 400 mg/l. The percentage adsorption and distribution coefficients (K d ) were determined for the adsorption system as a function of sorbate concentration. In the ion exchange evaluation part of the study, it is determined that in every concentration range, adsorption ratios of clinoptilolite metal cations match to Langmuir, Freundlich, and Dubinin Kaganer Radushkevich (DKR) adsorption isotherm data, adding to that every cation exchange capacity metals has been calculated. It was found that the adsorption phenomena depend on charge density and hydrated ion diameter. According to the equilibrium studies, the selectivity sequence can be given as Co 2+ > Cu 2+ > Zn 2+ > Mn 2+. These results show that natural zeolites hold great potential to remove cationic heavy metal species from industrial wastewater Elsevier Inc. All rights reserved. Keywords: Adsorption; Wastewaters; Heavy metals; Natural zeolites; Clinoptilolite 1. Introduction Many toxic heavy metals have been discharged into the environment as industrial wastes, causing serious soil and water pollution . Pb +2,Cu +2,Fe +3,andCr +3 are especially common metals that tend to accumulate in organisms, causing numerous diseases and disorders . Theyarealso common groundwater contaminants at industrial and military installations. Numerous processes exist for removing dissolved heavy metals, including ion exchange, precipitation, phytoextraction, ultrafiltration, reverse osmosis, and electrodialysis [3 6]. The use of alternative low-cost materials as potential sorbents for the removal of heavy metals has been emphasized recently. Activated carbon adsorption is considered to be a particularly competitive and effective process for the removal of heavy metals at trace quantities ; however, the use of ac- * Corresponding author. Fax: address: (R. Donat). tivated carbon is not suitable in developing countries due to the high costs associated with production and regeneration of spent carbon . Various treatment processes are available, among which ion exchange is considered to be cost-effective if low-cost ion exchangers such as zeolites are used . Zeolites are naturally occurring hydrated aluminosilicate minerals. They belong to the class of minerals known as tectosilicates. Most common natural zeolites are formed by alteration of glass-rich volcanic rocks (tuff) with fresh water in playa lakes or by seawater . The structures of zeolites consist of three-dimensional frameworks of SiO 4 and AlO 4 tetrahedra. The aluminum ion is small enough to occupy the position in the center of the tetrahedron of four oxygen atoms, and the isomorphous replacement of Si 4+ by Al 3+ produces a negative charge in the lattice. The net negative charge is balanced by the exchangeable cation (sodium, potassium, or calcium). These cations are exchangeable with certain cations in solutions such as lead, cadmium, zinc, and manganese [11,12]. The fact that zeolite exchangeable /$ see front matter 2004 Elsevier Inc. All rights reserved. doi: /j.jcis
2 310 E. Erdem et al. / Journal of Colloid and Interface Science 280 (2004) ions are relatively innocuous (sodium, calcium, and potassium ions) makes them particularly suitable for removing undesirable heavy metal ions from industrial effluent waters. One of the earliest applications of a natural zeolite was in removal and purification of cesium and strontium radioisotopes . Clinoptilolite is the most abundant natural zeolite and has the chemical formula Na 0.1 K 8.57 Ba 0.04 (Al 9.31 Si O 72 ) 19.56H 2 O . Its characteristic tabular morphology shows an open reticular structure of easy access, formed by open channels of 8- to 10-membered rings . Considerable research has been conducted to characterize the chemical, surface, and ion-exchange properties of clinoptilolite [15 19]. The ion-exchange capacity of natural zeolite (clinoptilolite) for inorganic cations has been investigated by many authors [20,21]. The selectivity series of clinoptilolite in the sodium form was determined by Zamzow et al., as follows: Pb 2+ > Cd 2+ > Cs + > Cu 2+ > Co 2+ > Cr 3+ > Zn 2+ > Ni 2+ > Hg 2+ . Jama and Yücel observed that clinoptilolite shows a very high preference for ammonium ions over sodium and calcium but not over potassium . Mieret al. described the interactions of Pb 2+,Cd 2+,andCr 3+ competing for ion-exchange sites in natural clinoptilolite . Inglezakis et al. studied the ion exchange of Pb 2+,Cu 2+, Fe 3+,andCr 3+ on natural clinoptilolite and showed that equilibrium is favorable for Pb 2+, unfavorable for Cu 2+,and of sigmoid shape for Cr 3+ and Fe 3+ . As seen from the literature review, zeolites can be used for the removal of some heavy metals from wastewater. The clinoptilolite samples from different regions show different behavior in ion-exchange processes. In this study, the adsorption properties of the natural zeolite (Clinoptillolite, Western Anatolian) with respect to some heavy metal cations in solution were investigated. 2. Materials and methods 2.1. Zeolite source and conditioning Samples of zeolite were taken from the Enli Mining Company open pit mine in Manisa-Gördes in Western Anatolia. The crushed original zeolite was ground and passed through µm sieves and was dried in an oven at 100 ± 5 C for 24 h. It was characterized by X-ray diffraction (XRD) and chemical analysis. Chemical composition of zeolite samples was determined by the usual analytical methods for silicate materials. Standard wet chemical analysis, along with instrumental methods, was adopted . Al 2 O 3,Fe 2 O 3, CaO, and MgO were analyzed with titrimetric methods and SiO 2 was analyzed with gravimetric methods. Na 2 OandK 2 O were found out by flame photometry. The results of the chemical analyses are presented in Table 1. Table 1 Chemical composition and physical properties of natural zeolite sample (wt%) Chemical composition (%) Physical properties SiO Appearance porosity (%), 41.5 Al 2 O Appearance density (g/cm 3 ), 2.27 Fe 2 O Weight of per unit volume (g/cm 3 ), 1.32 CaO 2.07 Water absorption (original) (%), 31.3 MgO 1.13 Water absorption (grinding) (%), Na 2 O 0.52 Oil absorption (g oil/100 g sample), 51 K 2 O 2.83 Whiteness (%), 68 SO Original bleaching (g sample/g tonsil), 1.95 H 2 O 6.88 Active bleaching (g sample/g tonsil), 1.92 Si/Al 4.66 ph Reagents Inorganic chemicals were supplied by Merck as analytical-grade reagents and deionized water was used. The metal ions studied were Co(II), Cu(II), Zn(II), and Mn(II). We prepared a synthetic stock solution of copper, manganese, and cobalt using their nitrate salts, Cu(NO 3 ) 2 3H 2 O, Mn(NO 3 ) 2 4H 2 O, and Co(NO 3 ) 2 6H 2 O, respectively, in deionized water. The stock solution of Zn(II) was prepared using ZnCl 2 salts Batch adsorption studies The ion exchange of heavy metals on natural zeolite was carried out using the batch method. Batch adsorption experiments were conducted using 10 g of adsorbent with 500 ml of solutions containing heavy metal ions of desired concentrations at constant temperatures (25 C) in 500-ml plastic bottles. The particle size of the sample (clinoptilolite) used was in the range of µm. The bottles were shaken in a sieve for 5.5 h and solutions containing heavy metals were filtered through Whatman filter paper (No. 42). The exact concentration of metal ions and filterable metal concentrations were determined by AAS (ATI UNICAM 929 atomic absorption spectrophotometer). The flame type was air acetylene and absorption wavelengths are Cu 2+ (324.7 nm), Zn 2+ (213.9 nm), Co 2+ (240.7 nm), and Mn 2+ (279.5 nm). The percent adsorption (%) and distribution ratio (K d ) were calculated using the equations % adsorption = C i C f 100, (1) C f where C i and C f are the concentrations of the metal ion in initial and final solutions, and respectively, and amount of metal in adsorbent K d = (2) amount of metal in solution V m ml/g, where V is the volume of the solution (ml) and m is the weight of the adsorbent (g).
3 E. Erdem et al. / Journal of Colloid and Interface Science 280 (2004) Fig. 1. Adsorption of metal ions by natural zeolite sample as a function of initial concentration: m = 10 g, V = 500 ml, ph 6 7, time 5.5 h. The percent adsorption and K d (ml/g) can be correlated by the following equation : % adsorption = 100K d K d + V/m. 3. Results and discussion 3.1. Properties of natural zeolites A chemical analysis of the treated zeolite is presented in Table 1. This study showed that natural zeolite contained a complement of exchangeable sodium, potassium, and calcium ions. The Si/Al ratio is 4.66 (mol/mol) and the corresponding ratio of (Na + K)/Ca is The chemical composition, the theoretical exchange capacity, and the Si/Al ratio, generally ranging from 4 to 5.5, are typical for clinoptilolite [28 30]. Low-silica members are enriched with calcium, whereas high-silica clinoptilolites are enriched with potassium, sodium, and magnesium. It was found that the natural zeolite contains approximately 70% clinoptilolite and plagioclase, mica, quartz, smectite, and K-feldsparchlorite minerals by XRD analysis Adsorption of metals on natural zeolite The adsorption of Cu 2+,Co 2+,Zn 2+,andMn 2+ onto natural zeolite as a function of their concentrations was studied at 30 C by varying the metal concentration from 100 to 400 mg/l while keeping all other parameters constant. The results are shown in Figs. 1 and 2. Percentage adsorption for Cu 2+,Co 2+,Zn 2+,andMn 2+ decreases with increasing metal concentration in aqueous solutions. These results indicate that energetically less favorable sites become involved with increasing metal concentrations in the aqueous (3) Fig. 2. Variation of metal ions on natural zeolite as a function of initial concentration: m = 10 g, V = 500 ml, ph 6 7, time 5.5 h. solution. The heavy metal uptake is attributed to different mechanisms of ion-exchange processes as well as to the adsorption process. During the ion-exchange process, metal ions had to move through the pores of the zeolite mass, but also through channels of the lattice, and they had to replace exchangeable cations (mainly sodium and calcium). Diffusion was faster through the pores and was retarded when the ions moved through the smaller diameter channels. In this case the metal ion uptake could mainly be attributed to ion-exchange reactions in the microporous minerals of the zeolite samples. Fig. 2 illustrates K d as a function of metal ions concentrations. The K d values increase with the decreasing concentration of metal ions. In other words, the K d values increase as dilution of metal ions in solution proceeds. These results indicate that energetically less favorable sites become involved with increasing metal concentration in the aqueous solution. The maximal exchange levels attained were as follows: Cu %, Co %, Zn %, and Mn % Isotherm models The sorption data have been subjected to different sorption isotherms, namely, Langmuir, Freundlich, and Dubinin Kaganer Radushkevich (DKR). The equilibrium data for metal cations over the concentration range from 100 to 400 mg/l at30 C have been correlated with the Langmuir isotherm : C e /C ads = 1/Qb + C e /Q, where C e is the equilibrium concentration of metal in solution (M), C ads is the number of metal ions sorbed onto zeolite, and Q and b are Langmuir constants related to sorption capacity and sorption energy, respectively. Maximum sorption capacity (Q) represents monolayercoverageof sorbent with sorbate and b represents enthalpy of sorption and should vary with temperature. A linear plot is obtained when (4)
4 312 E. Erdem et al. / Journal of Colloid and Interface Science 280 (2004) Table 2 Characteristic parameters and determination coefficient of the experimental data according to the Langmuir equation Metal Q (mmol/kg) b (l/g) R 2 Cu Co Zn Mn C e /C ads is plotted against C e over the entire concentration range of metal ions investigated. The Langmuir model parameters and the statistical fits of the sorption data to this equation are given in Table 2. The Langmuir model effectively described the sorption data with all R 2 values >0.95. According to the Q (mmol/kg) parameter, sorption on zeolite is produced following the sequence Co 2+ > Cu 2+ > Zn 2+ > Mn 2+. Zeolites, in general, are weakly acidic in nature and sodium-form exchangers are selective for hydrogen (R Na+ H 2 O RH + Na + + OH ), which leads to high ph values when the exchanger is equilibrated with relatively dilute electrolyte solutions , making metal hydroxide precipitation feasible. In natural zeolites these metals seem to reach saturation, which means that the metal had filled possible available sites and further adsorption could take place only at new surfaces. Ion-exchange capacity of heavy metal cations listed in Table 2 indicates the following selectivity sequence: Co 2+ > Cu 2+ > Zn 2+ > Mn 2+. The heavy metal cations are present as hexaaqua complex ions with six surrounding water molecules in the solution and they passed the channel of zeolite in this form . Since the adsorption phenomena depend on the charge density of cations, the diameter of hydrate cations is very important. The charges of the metal cation are the same (+2); therefore Mn 2+ ions (the biggest diameter) have minimum adsorption, and Co 2+ ions (the least diameter) have maximum adsorption. The Langmuir model effectively described the sorption data with all R 2 values >0.95, according to the b (mmol/g) parameter. Sorption on natural zeolite is produced following the sequence Co 2+ > Cu 2+ > Zn 2+ > Mn 2+. The high Si/Al ratio of clinoptilolite results in a typical low anionic field that gives rise to good selectivity. The Freundlich sorption isotherm, one of the most widely used mathematical descriptions, usually fits the experimental data over a wide range of concentrations. This isotherm gives an expression encompassing the surface heterogeneity and the exponential distribution of active sites and their energies. The Freundlich adsorption isotherms were also applied to the removal of Co 2+,Cu 2+,Zn 2+,andMn 2+ on zeolite (Fig. 3), log C ads = log K + 1/nlogC e, where C e is the equilibrium concentration in mg/l andc ads shows that the adsorption seems to follow the Freunlich (5) Fig. 3. Freundlich plots for metal ions adsorption onto natural zeolite. Table 3 Freundlich adsorption equations and constants (log k and n) for metal cations on natural zeolite Metal log k (mg/g) 1/n R 2 Cu Co Zn Mn isotherm model as well as the Langmuir isotherm. The constants K and n were calculated for each cation (Table 3). K is a parameter related to the temperature and n is a characteristic constant for the adsorption system under study. Values of n between 2 and 10 shows good adsorption. The numerical value of 1/n < 1 indicates that adsorption capacity is only slightly suppressed at lower equilibrium concentrations. This isotherm does not predict any saturation of the sorbent by the sorbate; thus infinite surface coverage is predicted mathematically, indicating multilayer adsorption on the surface . The Dubinin Kaganer Radushkevich (DKR) has been used to describe the sorption of metal ions on clays. The DKR equation has the form ln C ads = ln X m βε 2, where C ads is the number of metal ions adsorbed per unit weight of adsorbent (mg/g), X m is the maximum sorption capacity, β is the activity coefficient related to mean sorption energy, and ε is the Polanyi potential, which is equal to ε = RT ln(1 + 1/C e ), where R is the gas constant (kj mol 1 K 1 )andt is the temperature (K). The saturation limit X m may represent the total specific micropore volume of the sorbent. The sorption potential is independent of the temperature but varies according to the nature of sorbent and sorbate . The slope of the plot of ln C ads versus ε gives β (mol 2 /J 2 ) and the intercept yields the sorption capacity, X m (mg/g). The sorption space (6) (7)
5 E. Erdem et al. / Journal of Colloid and Interface Science 280 (2004) in the vicinity of a solid surface is characterized by a series of equipotential surfaces having the same sorption potential. This sorption potential is independent of the temperature but varies according to the nature of sorbent and sorbate. The sorption energy can also be worked out using the following relationship: E = 1/ 2β. The plot of ln C ads against ε 2 for metal ion sorption on natural zeolite is shown in Fig. 4. The DKR parameters are calculated from the slope of the line in Fig. 4 and listed in Table 4.AsshowninTable 4,theE values are for Cu 2+, for Co 2+,9.77forZn 2+, and 8.81 kj/mol for Mn 2+ on the natural zeolite. They are the orders of an ion-exchange mechanism, in which the sorption energy lies within 8 16 kj/mol [34,35]. The sorption capacity X m in the DKR equation is found to be 0.22 for Cu 2+,0.50forCo 2+, 0.29 for Zn 2+, and 0.15 mmol/kg for Mn Summary It was considered that the metal cations are formed as high-spin aqua complexes and the hydrate ion diameter is the same as the diameter of aqua-complex ions. The diameters of hydrated ions are given as r Mn >r Zn >r Cu >r Co in the literature . If the ionic radii are compared with the free dimensions of the clinoptilolite channels, it is apparent that all of the unhydrated ions can pass readily through the channels, but Fig. 4. DRK plots of metal ions on natural zeolite at constant temperature. (8) since the hydrated ions are approximately the same size as the channel dimensions, they may exchange only with difficulty. It follows that for exchange to take place, at least some of the waters of hydration must be stripped from the solvated ions . The DKR and Langmuir equations were used to describe the sorption isotherms of single-solute systems. The sorption energy E determined in the DKR equation (11.95 for Cu 2+, for Co 2+,9.77forZn 2+, and 8.81 kj/mol for Mn 2+ ) revealed the nature of the ion-exchange mechanism in both systems. The sorption isotherms of binary solute systems could be fitted by the competitive Langmuir model, where the Langmuir parameters were directly adopted from those obtained in single-solute systems. These results show that natural zeolite can be used effectively for the removal of metal cations from wastewater. This naturally occurring material provides a substitute for the use of activated carbon as adsorbent due to its availability and its low cost. References  S.H. Lin, R.S. Juang, J. Hazard. Mater. B 92 (2002) 315.  V.J. Inglezakis, M.D. Loizidou, H.P. Grigoropoulou, J. Colloid Interface Sci. 261 (2003) 49.  L.E. Applegate, Chem. Eng. 91 (1984) 64.  A.K. Sengupta, D. Clifford, Environ. Sci. Technol. 20 (1986) 149.  J. Geselbarcht, Micro Filtration/Reverse Osmosis Pilot Trials for Livermore, California, Advanced Water Reclamation, in: 1996 Water Reuse Conference Proceedings, AWWA, 1996, p  J.L. Schnoor, Phytoremediation, TE-97-01, Ground-Water Remediation Technologies Analysis Center, Pittsburgh,  C.P. Huang, D.W. Blankenship, Water Res. 18 (1984) 37.  K.K. Panday, G. Parsed, V.N. Singh, Water Res. 19 (1985) 869.  S.E. Bailey, T.J. Olin, R.M. Bricka, D.D. Adrian, Water Res. 33 (1999)  V. Badillo-Almaraz, P. Trocellier, I. Davila-Rangel, Nucl. Instrum. Methods Phys. Res. B 210 (2003) 424.  R.M. Barer, Zeolites and Clay Minerals as Sorbent and Molecular Sieves, Academic Press, New York,  D.W. Breck, J. Chem. Edu. 41 (1964) 678.  M.B. Hafez, A.F. Nazmy, F. Salem, M. Eldesoki, J. Radioanal. Chem. 47 (1978) 115.  E. Galli, G. Gottardi, H. Mayer, A. Preisinger, E. Passaglia, Acta Crystallogr. Sect. B 39 (1983) 189.  K.D. Mondale, R.M. Carland, F.F. Aplan, Miner. Eng. 8 (1995) 535.  M.J. Semmens, M. Seyfarth, in: An International Conference on the Occurrence, Properties and Utilization of Natural Senilities, Tucson, AZ, 1976, p  M.W. Ackley, R. Yang, AlChE J. 37 (1991)  M.J. Zamzow, J.E. Murphy, Sep. Sci. Technol. 27 (1992) Table 4 Parameter obtained in the DKR equation DKR Cu 2+ Co 2+ Zn 2+ Mn 2+ X m (mmol/kg) β (mol 2 /J 2 ) Sorption energy (E,kJ/mol) Correlation coefficient, R
6 314 E. Erdem et al. / Journal of Colloid and Interface Science 280 (2004)  R.M. Carland, F.F. Aplan, Miner. Metall. Process. 11 (1995) 210.  M.S. Joshi, R.P. Mohan, J. Colloid Interface Sci. 95 (1983) 131.  G. Blanchard, M. Maunaye, G. Martin, Water Res. 18 (1984)  M.J. Zamzow, B.R. Eichbaum, K.R. Sandgren, D.E. Shanks, Sep. Sci. Technol. 25 (1990)  M.A. Jama, H. Yücel, Sep. Sci. Technol. 24 (15) (1990)  M.V. Mier, R.L. Callejas, R. Gehr, B.E.J. Cisneros, P.J.J. Alvarez, Water Res. 35 (2) (2001) 373.  V.J. Inglezakis, M.D. Loizidou, H.P. Grigoropoulou, Water Res. 36 (2002)  D.R. Corbin, B.F. Burgess, A.J. Vega, R.D. Farelee, Anal. Chem. 59 (1987)  S.A. Khan, U.R. Rehman, M.A. Khan, Waste Manage. 15 (1995) 271.  A. Langella, M. Pansini, P. Cappelletti, B. de Gennaro, M. de Gennaro, C. Colella, Micropor. Mesopor. Mater. 37 (2000) 337.  M. Loizidou, K.J. Haralambous, A. Loukatos, D. Dimitrakopoulou, J. Environ. Sci. Health A 27 (1992)  E. Malliou, M. Malamis, P.O. Sakellarides, Water Sci. Technol. 25 (1992) 133.  I. Langmuir, J. Am. Chem. Soc. 40 (1918)  H. Leinonen, J. Lehto, Waste Manage. Res. 19 (2001) 45.  S.M. Hasany, M.M. Saeed, M. Ahmed, J. Radioanal. Nucl. Chem. 252 (2002) 477.  F. Helferrich, Ion Exchange, McGraw Hill, New York,  W. Rieman, H. Walton, Ion Exchange in Analytical Chemistry, in: International Series of Monographs in Analytical Chemistry, vol. 38, Pergamon, Oxford,  S. Özkar, N.K. Tunalı, Anorganik Kimya, Gazi Üniversitesi, Ankara, 1997, p  M.J. Semmens, W.P. Martin, Water Res. 22 (1988) 537.
i Acid-base Chemistry of Aquatic Systems An introduction to the chemistry of acid-base equilibria with emphasis on the carbon dioxide system in natural waters eith A. Hunter Professor in Chemistry Department
Synthesis of mesoporous silica particles with control of both pore diameter and particle size Master of Science Thesis in Materials and Nanotechnology program ALBERT BARRABINO Department of Chemical and
A R C H I V E S O F M E T A L L U R G Y A N D M A T E R I A L S Volume 55 2010 Issue 2 A. ŠTRKALJ, A. RADENOVIĆ,J.MALINA THE USE OF METALLURGICAL WASTE MATERIAL FROM ALUMINIUM PRODUCTION FOR THE REMOVAL
Unit 8 Chemical Equilibrium Focusing on Acid-Base Systems unit 8Chemical Equilibrium Chemical Equilibrium Focusing on Acid Base Systems Equilibrium describes any condition or situation of balance. We recognize
2192 J. Phys. Chem. B 2005, 109, 2192-2202 High-Surface-Area Catalyst Design: Synthesis, Characterization, and Reaction Studies of Platinum Nanoparticles in Mesoporous SBA-15 Silica R. M. Rioux, H. Song,
United States Environmental Protection Agency Office of Water 4304 EPA-822-R-01-005 March 2001 Streamlined Water-Effect Ratio Procedure for Discharges of Copper Streamlined Water-Effect Ratio Procedure
J. Phys. Chem. B 1998, 102, 10347-10358 10347 Precision Relative Aggregation Number Determinations of SDS Micelles Using a Spin Probe. A Model of Micelle Surface Hydration Barney L. Bales,* Luis Messina,
Reaction of Aluminum with Water to Produce Hydrogen A Study of Issues Related to the Use of Aluminum for On-Board Vehicular Hydrogen Storage U.S. Department of Energy Page 1 of 26 CONTENTS EXECUTIVE SUMMARY..
GE Healthcare High-throughput Process Development with PreDictor Plates Principles and Methods imagination at work Handbooks from GE Healthcare GST Gene Fusion System Handbook 18-1157-58 Affinity Chromatography
Acid-base Equilibria and Calculations A Chem1 Reference Text Stephen K. Lower Simon Fraser University Contents 1 Proton donor-acceptor equilibria 4 1.1 The ion product of water... 4 1.2 Acid and base strengths...
AS/A Level GCE GCE Chemistry A OCR Advanced Subsidiary GCE in Chemistry A H034 OCR Advanced GCE in Chemistry A H434 version 4 September 2013 QAN 500/2425/5 QAN 500/2347/0 Contents 1 About these Qualifications
DOE-HDBK-1019/2-93 JANUARY 1993 DOE FUNDAMENTALS HANDBOOK NUCLEAR PHYSICS AND REACTOR THEORY Volume 2 of 2 U.S. Department of Energy Washington, D.C. 20585 FSC-6910 Distribution Statement A. Approved for
Radioactive Waste Management Glossary 2003 Edition RADIOACTIVE WASTE MANAGEMENT GLOSSARY 2003 Edition The following States are Members of the International Atomic Energy Agency: AFGHANISTAN ALBANIA ALGERIA
All Biochars are Not Created Equal, and How to Tell Them Apart Version 2 (October 2009), which supercedes the digital reprint issued at the North American Biochar Conference, Boulder, CO August 2009 Hugh
Process monitoring in biogas plants Bernhard Drosg Technical Brochure written by: Bernhard Drosg Copyright 2013 IEA Bioenergy. All rights reserved. First electronic edition produced in 2013 A catalogue
Bulletin 945 Authors Liming Chen Research Associate School of Environment and Natural Resources The Ohio State University Warren A. Dick Professor School of Environment and Natural Resources The Ohio State
GUIDANCE DOCUMENT DEVELOPMENT OF SITE-SPECIFIC IMPACT TO GROUND WATER SOIL REMEDIATION STANDARDS USING THE SYNTHETIC PRECIPITATION LEACHING PROCEDURE Version 3.0 - November 2013 New Jersey Department of
Water Research 37 (2003) 1469 1487 Review Ozonation of drinkingwater: Part II. Disinfection and by-product formation in presence of bromide, iodide or chlorine Urs von Gunten* Swiss Federal Institute for
The Other CO 2 -Problem Eight Experiments for Students and Teachers introduction Ocean Acidification - The Other CO 2 Problem The oceans cover more than two-thirds of the planet earth. This vast body of
Field Estimation of Soil Water Content A Practical Guide to Methods, Instrumentation and Sensor Technology VIENNA, 2008 TRAINING COURSE SERIES30 TRAINING COURSE SERIES No. 30 Field Estimation of Soil Water
Arsenic in Groundwater in the Surrey-Langley Area Julie Wilson, Hans Schreier and Sandra Brown Institute for Resources & Environment The University of British Columbia For: Fraser Health Authority Environmental
Chapter 3 - Radioactive Decay Kinetics The number of nuclei in a radioactive sample that disintegrate during a given time interval decreases exponentially with time. Because the nucleus is insulated by
WHO/FCH/CAH/06.1 For further information please contact: Department of Child and Adolescent Health and Development (CAH) World Health Organization 20 Avenue Appia 1211 Geneva 27 Switzerland fax + 41 22
Chem. Rev. 1990, 90. 33-72 93 The Sol-Gel Process LARRY L. HENCH' and JON K. WEST Dq"nt of Materials Sc*mce and Enghwrhg, Advanced Materials Research Center, UnimrMy of Floryle. oakresville. Fknm 326 11
From End-of-Pipe Technology to Clean Technology: Effects of Environmental Regulation on Technological Change in the Chlor-Alkali Industry in Japan and Western Europe PROEFSCHRIFT ter verkrijging van de
Energy and Environmental Systems Group Institute for Sustainable Energy, Environment and Economy (ISEEE) WABAMUN AREA CO 2 SEQUESTRATION PROJECT (WASP) Author Runar Nygaard Rev. Date Description Prepared
Non-Volatile Memory Based on Solid Electrolytes Michael N. Kozicki, Chakravarthy Gopalan, Murali Balakrishnan, Mira Park, and Maria Mitkova Center for Solid State Electronics Research Arizona State University